LMucko/crystallography-open-database huggingface dataset:
Effect of Mo doping on the room-temperature structure of vanadium sesquioxide
Tenailleau, C.; Suard, E.; Rodriguez-Carvajal, J.; Crosnier-Lopez, M.P.; Lacorre, P.; Chemistry of Materials (1,1989-) 14 (2002) 3569–3575; doi:

data_4002538
_publ_section_title
;
 Effect of Mo doping on the room-temperature structure of vanadium
 sesquioxide
;
_journal_name_full               'Chemistry of Materials (1,1989-)'
_journal_page_first              3569
_journal_page_last               3575
_journal_volume                  14
_journal_year                    2002
_chemical_formula_sum            'Mo0.2 O3 V1.8'
_chemical_name_systematic        '(V0.9 Mo0.1)2 O3'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.9405
_cell_length_b                   4.9405
_cell_length_c                   14.1631
_cell_volume                     299.385
_citation_journal_id_ASTM        CMATEX
_cod_data_source_file            Tenailleau_CMATEX_2002_242.cif
_cod_data_source_block           Mo0.2O3V1.8
_cod_original_cell_volume        299.3855
_cod_database_code               4002538
Refinement of crystal structure of Na2 H2 P2 O7 using X-ray powder diffraction data
Selevich, K.A.; Ivashkevich, L.S.; Selevich, A.F.; Lyakhov, A.S.; Zhurnal Neorganicheskoi Khimii 47 (2002) 1672–1675; doi:

data_1532236
_publ_section_title
;
 Refinement of crystal structure of Na2 H2 P2 O7 using X-ray powder
 diffraction data
;
_journal_name_full               'Zhurnal Neorganicheskoi Khimii'
_journal_page_first              1672
_journal_page_last               1675
_journal_volume                  47
_journal_year                    2002
_chemical_formula_sum            'H2 Na2 O7 P2'
_chemical_name_systematic        'Na2 (H2 P2 O7)'
_space_group_IT_number           70
_symmetry_space_group_name_Hall  '-F 2uv 2vw'
_symmetry_space_group_name_H-M   'F d d d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   27.521
_cell_length_b                   12.3519
_cell_length_c                   6.8597
_cell_volume                     2331.863
_citation_journal_id_ASTM        ZNOKAQ
_cod_data_source_file            Selevich_ZNOKAQ_2002_1252.cif
_cod_data_source_block           H2Na2O7P2
_cod_original_cell_volume        2331.864
_cod_database_code               1532236
Structural characterization of neptunyl(VI) trinitrato complexes: M[NpO~2~(NO~3~)~3~] (M = NH~4~^+^ and K^+^)
Wang, Junhu; Kitazawa, Takafumi; Nakada, Masami; Yamashita, Toshiyuki; Takeda, Masuo; Bulletin of the Chemical Society of Japan 75 (2002) 253–257; doi:10.1246/bcsj.75.253

data_1532237
_publ_section_title
;
 Structural characterization of neptunyl(VI) trinitrato complexes:
 M[NpO~2~(NO~3~)~3~] (M = NH~4~^+^ and K^+^)
;
_journal_issue                   2
_journal_name_full               'Bulletin of the Chemical Society of Japan'
_journal_page_first              253
_journal_page_last               257
_journal_paper_doi               10.1246/bcsj.75.253
_journal_volume                  75
_journal_year                    2002
_chemical_formula_sum            'K N3 Np O11'
_chemical_name_systematic        'K (Np O2) (N O3)3'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   9.22
_cell_length_b                   9.22
_cell_length_c                   18.76
_cell_volume                     1381.101
_citation_journal_id_ASTM        BCSJA8
_cod_data_source_file            Wang_BCSJA8_2002_1112.cif
_cod_data_source_block           K1N3Np1O11
_cod_original_formula_sum        'K1 N3 Np1 O11'
_cod_database_code               1532237
Effect of Mo doping on the room-temperature structure of vanadium sesquioxide
Tenailleau, C.; Lacorre, P.; Suard, E.; Rodriguez-Carvajal, J.; Crosnier-Lopez, M.P.; Chemistry of Materials (1,1989-) 14 (2002) 3569–3575; doi:

data_4002539
_publ_section_title
;
 Effect of Mo doping on the room-temperature structure of vanadium
 sesquioxide
;
_journal_name_full               'Chemistry of Materials (1,1989-)'
_journal_page_first              3569
_journal_page_last               3575
_journal_volume                  14
_journal_year                    2002
_chemical_formula_sum            'Mo0.4 O3 V1.6'
_chemical_name_systematic        '(V0.8 Mo0.2)2 O3'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.9309
_cell_length_b                   4.9309
_cell_length_c                   14.2819
_cell_volume                     300.725
_citation_journal_id_ASTM        CMATEX
_cod_data_source_file            Tenailleau_CMATEX_2002_243.cif
_cod_data_source_block           Mo0.4O3V1.6
_cod_original_cell_volume        300.7247
_cod_database_code               4002539
Magnetic Structures and Properties of Cr1-t Fet As
Selte, K.; Fjellvag, H.; Kjekshus, A.; Andresen, A.F.; Acta Chemica Scandinavica, Series A: (28,1974-) 33 (1979) 727–731; doi:

data_1532238
_publ_section_title
;
 Magnetic Structures and Properties of Cr1-t Fet As
;
_journal_name_full
'Acta Chemica Scandinavica, Series A: (28,1974-)'
_journal_page_first              727
_journal_page_last               731
_journal_volume                  33
_journal_year                    1979
_chemical_formula_sum            'As Cr0.5 Fe0.5'
_chemical_name_systematic        'Cr.5 Fe.5 As'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.5287
_cell_length_b                   3.3899
_cell_length_c                   6.132
_cell_volume                     114.924
_citation_journal_id_ASTM        ACAPCT
_cod_data_source_file            Selte_ACAPCT_1979_1997.cif
_cod_data_source_block           As1Cr0.5Fe0.5
_cod_original_cell_volume        114.9243
_cod_original_formula_sum        'As1 Cr0.5 Fe0.5'
_cod_database_code               1532238
Non-aqueous synthesis and structure of a novel monodimensional zirconium phosphate : (N H4)3 (Zr (O H)2 (P O4) (H P O4))
Wang, D.; Yu, R.; Kajiyoshi, K.; Takei, T.; Onda, A.; Yanagisawa, K.; Kinomura, N.; Kumada, N.; Chemistry Letters 2002 (2002) 398–399; doi:

data_8000217
_publ_section_title
;
 Non-aqueous synthesis and structure of a novel monodimensional zirconium
 phosphate : (N H4)3 (Zr (O H)2 (P O4) (H P O4))
;
_journal_name_full               'Chemistry Letters'
_journal_page_first              398
_journal_page_last               399
_journal_volume                  2002
_journal_year                    2002
_chemical_formula_sum            'H15 N3 O10 P2 Zr'
_chemical_name_systematic        '(N H4)3 (Zr (O H)2 (P O4) (H P O4))'
_space_group_IT_number           1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_cell_angle_alpha                91.85
_cell_angle_beta                 92.16
_cell_angle_gamma                74.25
_cell_formula_units_Z            2
_cell_length_a                   8.1432
_cell_length_b                   12.718
_cell_length_c                   5.2463
_cell_volume                     522.426
_citation_journal_id_ASTM        CMLTAG
_cod_data_source_file            Wang_CMLTAG_2002_1132.cif
_cod_data_source_block           H15N3O10P2Zr1
_cod_original_formula_sum        'H15 N3 O10 P2 Zr1'
_cod_database_code               8000217
Structural study of the cation ordering in the ternary oxide Ba8 Ti3 Nb4 O24
Teneze, N.; Boullay, P.; Petricek, V.; Trolliard, G.; Mercurio, D.; Solid State Sciences 4 (2002) 1129–1136; doi:

data_1532239
_publ_section_title
;
 Structural study of the cation ordering in the ternary oxide Ba8 Ti3 Nb4
 O24
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              1129
_journal_page_last               1136
_journal_volume                  4
_journal_year                    2002
_chemical_formula_sum            'Ba8 Nb4 O24 Ti3'
_chemical_name_systematic        'Ba8 (Ti3 Nb4 O24)'
_space_group_IT_number           193
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   10.068
_cell_length_b                   10.068
_cell_length_c                   18.917
_cell_volume                     1660.616
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Teneze_SSSCFJ_2002_892.cif
_cod_data_source_block           Ba8Nb4O24Ti3
_cod_database_code               1532239
Hydrothermal synthesis, structure determination from powder data of a three-dimensional zirconium diphosphonate with an exceptionally high thermal stability : Zr (O3 P - (C H2) - P O3) or MIL-57
Serre, C.; Ferey, G.; Journal of Materials Chemistry 12 (2002) 2367–2369; doi:

data_7222221
_publ_section_title
;
 Hydrothermal synthesis, structure determination from powder data of a
 three-dimensional zirconium diphosphonate with an exceptionally high
 thermal stability : Zr (O3 P - (C H2) - P O3) or MIL-57
;
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              2367
_journal_page_last               2369
_journal_volume                  12
_journal_year                    2002
_chemical_formula_sum            'C H2 O6 P2 Zr'
_chemical_name_systematic        'Zr (O3 P (C H2) P O3)'
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 103.934
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.589
_cell_length_b                   8.11
_cell_length_c                   5.056
_cell_volume                     302.024
_citation_journal_id_ASTM        JMACEP
_cod_data_source_file            Serre_JMACEP_2002_1965.cif
_cod_data_source_block           C1H2O6P2Zr1
_cod_original_cell_volume        302.0237
_cod_original_formula_sum        'C1 H2 O6 P2 Zr1'
_cod_database_code               7222221
Structure and spin glass behaviour in non-metallic Yb2 Co Mn O6 perovskite manganite
Wang, X.-L.; James, M.; Horvat, J.; Gao, F.; Liu, H.K.; Dou, S.X.; Li, A.H.; Journal of Magnetism and Magnetic Materials 246 (2002) 86–92; doi:

data_1532240
_publ_section_title
;
 Structure and spin glass behaviour in non-metallic Yb2 Co Mn O6
 perovskite manganite
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              86
_journal_page_last               92
_journal_volume                  246
_journal_year                    2002
_chemical_formula_sum            'Co Mn O6 Yb2'
_chemical_name_systematic        'Yb2 ((Co Mn) O6)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.5594
_cell_length_b                   7.4154
_cell_length_c                   5.1825
_cell_volume                     213.649
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Wang_JMMMDC_2002_708.cif
_cod_data_source_block           Co1Mn1O6Yb2
_cod_original_cell_volume        213.6495
_cod_original_formula_sum        'Co1 Mn1 O6 Yb2'
_cod_database_code               1532240
Crystal structures and magnetic properties of zircon-type Lu1-x Yx Cr O4
Tezuka, K.; Doi, Y.; Hinatsu, Y.; Journal of Materials Chemistry 12 (2002) 1189–1193; doi:

data_7222222
_publ_section_title
;
 Crystal structures and magnetic properties of zircon-type Lu1-x Yx Cr O4
;
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              1189
_journal_page_last               1193
_journal_volume                  12
_journal_year                    2002
_chemical_formula_sum            'Cr Lu O4'
_chemical_name_systematic        'Lu (Cr O4)'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  'I 4bw 2bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a m d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.0186
_cell_length_b                   7.0186
_cell_length_c                   6.19
_cell_volume                     304.924
_citation_journal_id_ASTM        JMACEP
_cod_data_source_file            Tezuka_JMACEP_2002_1146.cif
_cod_data_source_block           Cr1Lu1O4
_cod_original_sg_symbol_Hall     '-I 4bd 2 (x+1/2,y+1/4,z+1/8)'
_cod_original_formula_sum        'Cr1 Lu1 O4'
_cod_database_code               7222222
Crystal structures of Na2 Zn P2 O7, K2 Zn P2 O7 and Li K Zn P2 O7 phases in the (M2 O) - (Zn O) - (P2 O5) glass-forming system (M = Li, Na and K)
Shepelev, Yu.F.; Petrova, M.A.; Novikova, A.S.; Lapshin, A.E.; Glass Physics and Chemistry 28 (2002) 317–321; doi:

data_1532241
_publ_section_title
;
 Crystal structures of Na2 Zn P2 O7, K2 Zn P2 O7 and Li K Zn P2 O7 phases
 in the (M2 O) - (Zn O) - (P2 O5) glass-forming system (M = Li, Na and K)
;
_journal_name_full               'Glass Physics and Chemistry'
_journal_page_first              317
_journal_page_last               321
_journal_volume                  28
_journal_year                    2002
_chemical_formula_sum            'Na2 O7 P2 Zn'
_chemical_name_systematic        'Na2 (Zn P2 O7)'
_space_group_IT_number           136
_symmetry_space_group_name_Hall  '-P 4n 2n'
_symmetry_space_group_name_H-M   'P 42/m n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.687
_cell_length_b                   7.687
_cell_length_c                   10.275
_cell_volume                     607.149
_citation_journal_id_ASTM        GPHCEE
_cod_data_source_file            Shepelev_GPHCEE_2002_1136.cif
_cod_data_source_block           Na2O7P2Zn1
_cod_original_cell_volume        607.1494
_cod_original_formula_sum        'Na2 O7 P2 Zn1'
_cod_database_code               1532241
Synthesis and characterization of a new layered gallium phosphate (Co (en)3) (Ga3 (H2 P O4)6 (H P O4)3) templated by cobalt complex
Wang, Y.; Xu, R.-R.; Yu, J.-H.; Shi, Z.; Journal of Solid State Chemistry 170 (2003) 176–181; doi:

data_1532242
_publ_section_title
;
 Synthesis and characterization of a new layered gallium phosphate (Co
 (en)3) (Ga3 (H2 P O4)6 (H P O4)3) templated by cobalt complex
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              176
_journal_page_last               181
_journal_volume                  170
_journal_year                    2003
_chemical_formula_sum            'C6 H39 Co Ga3 N6 O36 P9'
_chemical_name_systematic
;
(Co (N H2 (C H2)2 N H2)3) (Ga3 (H2 P O4)6 (H P O4)3)
;
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 108.278
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.2103
_cell_length_b                   22.0936
_cell_length_c                   9.5458
_cell_volume                     1844.457
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Wang_JSSCBI_2003_1465.cif
_cod_data_source_block           C6H39Co1Ga3N6O36P9
_cod_original_formula_sum        'C6 H39 Co1 Ga3 N6 O36 P9'
_cod_database_code               1532242
Crystal structures and magnetic properties of zircon-type Lu1-x Yx Cr O4
Tezuka, K.; Doi, Y.; Hinatsu, Y.; Journal of Materials Chemistry 12 (2002) 1189–1193; doi:

data_7222223
_publ_section_title
;
 Crystal structures and magnetic properties of zircon-type Lu1-x Yx Cr O4
;
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              1189
_journal_page_last               1193
_journal_volume                  12
_journal_year                    2002
_chemical_formula_sum            'Cr Lu0.75 O4 Y0.25'
_chemical_name_systematic        '(Lu0.75 Y0.25) (Cr O4)'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  'I 4bw 2bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a m d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.0448
_cell_length_b                   7.0448
_cell_length_c                   6.2085
_cell_volume                     308.123
_citation_journal_id_ASTM        JMACEP
_cod_data_source_file            Tezuka_JMACEP_2002_1147.cif
_cod_data_source_block           Cr1Lu0.75O4Y0.25
_cod_original_cell_volume        308.1229
_cod_original_sg_symbol_Hall     '-I 4bd 2 (x+1/2,y+1/4,z+1/8)'
_cod_original_formula_sum        'Cr1 Lu0.75 O4 Y0.25'
_cod_database_code               7222223
Crystal structures of Na2 Zn P2 O7, K2 Zn P2 O7 and Li K Zn P2 O7 phases in the (M2 O) - (Zn O) - (P2 O5) glass-forming system (M = Li, Na and K)
Shepelev, Yu.F.; Petrova, M.A.; Novikova, A.S.; Lapshin, A.E.; Glass Physics and Chemistry 28 (2002) 317–321; doi:

data_1532243
_publ_section_title
;
 Crystal structures of Na2 Zn P2 O7, K2 Zn P2 O7 and Li K Zn P2 O7 phases
 in the (M2 O) - (Zn O) - (P2 O5) glass-forming system (M = Li, Na and K)
;
_journal_name_full               'Glass Physics and Chemistry'
_journal_page_first              317
_journal_page_last               321
_journal_volume                  28
_journal_year                    2002
_chemical_formula_sum            'K2 O7 P2 Zn'
_chemical_name_systematic        'K2 (Zn P2 O7)'
_space_group_IT_number           136
_symmetry_space_group_name_Hall  '-P 4n 2n'
_symmetry_space_group_name_H-M   'P 42/m n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.858
_cell_length_b                   7.858
_cell_length_c                   11.322
_cell_volume                     699.113
_citation_journal_id_ASTM        GPHCEE
_cod_data_source_file            Shepelev_GPHCEE_2002_1137.cif
_cod_data_source_block           K2O7P2Zn1
_cod_original_cell_volume        699.1127
_cod_original_formula_sum        'K2 O7 P2 Zn1'
_cod_database_code               1532243
Mn substitution in the solid solution series Bi2 Pb8-x (P O4)6 O2-x. The crystal structure of Bi1.5 (Pb7.3 Mn0.7) (P O4)6 O1.3 a member of a new solid solution series Bi2-x Pb8 (P O4)6 O2-1.5x
Wang, S.; Lynch, V.; Steinfink, H.; Journal of Solid State Chemistry 173 (2003) 374–378; doi:

data_1532244
_publ_section_title
;
 Mn substitution in the solid solution series Bi2 Pb8-x (P O4)6 O2-x. The
 crystal structure of Bi1.5 (Pb7.3 Mn0.7) (P O4)6 O1.3 a member of a new
 solid solution series Bi2-x Pb8 (P O4)6 O2-1.5x
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              374
_journal_page_last               378
_journal_volume                  173
_journal_year                    2003
_chemical_formula_sum            'Bi1.47 Mn0.71 O25.32 P6 Pb7.29'
_chemical_name_systematic        'Bi1.47 (Pb7.29 Mn0.71) (P O4)6 O1.32'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   12.967
_cell_length_b                   10.294
_cell_length_c                   8.9994
_cell_volume                     1201.261
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Wang_JSSCBI_2003_1605.cif
_cod_data_source_block           Bi1.47Mn0.71O25.32P6Pb7.29
_cod_database_code               1532244
Crystal structures and magnetic properties of zircon-type Lu1-x Yx Cr O4
Tezuka, K.; Doi, Y.; Hinatsu, Y.; Journal of Materials Chemistry 12 (2002) 1189–1193; doi:

data_7222224
_publ_section_title
;
 Crystal structures and magnetic properties of zircon-type Lu1-x Yx Cr O4
;
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              1189
_journal_page_last               1193
_journal_volume                  12
_journal_year                    2002
_chemical_formula_sum            'Cr Lu0.5 O4 Y0.5'
_chemical_name_systematic        '(Lu0.5 Y0.5) (Cr O4)'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  'I 4bw 2bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a m d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.0682
_cell_length_b                   7.0682
_cell_length_c                   6.2234
_cell_volume                     310.918
_citation_journal_id_ASTM        JMACEP
_cod_data_source_file            Tezuka_JMACEP_2002_1148.cif
_cod_data_source_block           Cr1Lu0.5O4Y0.5
_cod_original_cell_volume        310.9177
_cod_original_sg_symbol_Hall     '-I 4bd 2 (x+1/2,y+1/4,z+1/8)'
_cod_original_formula_sum        'Cr1 Lu0.5 O4 Y0.5'
_cod_database_code               7222224
Crystal structures of Na2 Zn P2 O7, K2 Zn P2 O7 and Li K Zn P2 O7 phases in the (M2 O) - (Zn O) - (P2 O5) glass-forming system (M = Li, Na and K)
Shepelev, Yu.F.; Lapshin, A.E.; Petrova, M.A.; Novikova, A.S.; Glass Physics and Chemistry 28 (2002) 317–321; doi:

data_1532245
_publ_section_title
;
 Crystal structures of Na2 Zn P2 O7, K2 Zn P2 O7 and Li K Zn P2 O7 phases
 in the (M2 O) - (Zn O) - (P2 O5) glass-forming system (M = Li, Na and K)
;
_journal_name_full               'Glass Physics and Chemistry'
_journal_page_first              317
_journal_page_last               321
_journal_volume                  28
_journal_year                    2002
_chemical_formula_sum            'K Li O7 P2 Zn'
_chemical_name_systematic        'Li K (Zn P2 O7)'
_space_group_IT_number           26
_symmetry_space_group_name_Hall  'P 2c -2'
_symmetry_space_group_name_H-M   'P m c 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.36
_cell_length_b                   5.09
_cell_length_c                   10.26
_cell_volume                     645.481
_citation_journal_id_ASTM        GPHCEE
_cod_data_source_file            Shepelev_GPHCEE_2002_1139.cif
_cod_data_source_block           K1Li1O7P2Zn1
_cod_original_cell_volume        645.4813
_cod_original_formula_sum        'K1 Li1 O7 P2 Zn1'
_cod_database_code               1532245